LMucko/crystallography-open-database huggingface dataset:
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102294
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     'Pb2.952 Ba0.048 P2 O8'
_chemical_formula_structural     '(Pb0.984 Ba0.016)3 (PO4)2'
_chemical_formula_sum            'O8 P2 Pb3'
_chemical_formula_weight         811.54
_chemical_name_common            'Ba-doped lead phosphate'
_chemical_name_systematic        ' ?'
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            3
_cell_length_a                   5.4274(3)
_cell_length_b                   5.4274
_cell_length_c                   19.9933(14)
_cell_measurement_pressure       2620000.
_cell_measurement_temperature    298
_cell_volume                     510.03(5)
_cod_data_source_file            ws5002.cif
_cod_data_source_block           S4P35_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (362
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (50 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (362
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (50 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_Hall     -R32''-P3*2
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        'O8.00 P2 Pb3.00'
_cod_database_code               2102294
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102295
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     WC
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_chemical_formula_weight         195.86
_chemical_name_common            WC
_chemical_name_systematic        ' ?'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1
_cell_length_a                   2.8984(6)
_cell_length_b                   2.8984
_cell_length_c                   2.8288(10)
_cell_measurement_temperature    298
_cell_volume                     20.580(5)
_cod_data_source_file            ws5002.cif
_cod_database_code               2102295
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102296
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     Ni
_chemical_formula_moiety         Ni
_chemical_formula_structural     Ni
_chemical_formula_sum            Ni
_chemical_formula_weight         58.71
_chemical_name_common            Nickel
_chemical_name_systematic        ' ?'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   3.5433(9)
_cell_length_b                   3.5433
_cell_length_c                   3.5433
_cell_measurement_temperature    298
_cell_volume                     44.485(4)
_cod_data_source_file            ws5002.cif
_cod_database_code               2102296
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102297
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     'Pb2.952 Ba0.048 P2 O8'
_chemical_formula_structural     '(Pb0.984 Ba0.016)3 (PO4)2'
_chemical_formula_sum            'O8 P2 Pb3'
_chemical_formula_weight         811.54
_chemical_name_common            'Ba-doped lead phosphate'
_chemical_name_systematic        ' ?'
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            3
_cell_length_a                   5.4368(2)
_cell_length_b                   5.4368
_cell_length_c                   20.0175(10)
_cell_measurement_pressure       2370000.
_cell_measurement_temperature    298
_cell_volume                     512.42(3)
_cod_data_source_file            ws5002.cif
_cod_data_source_block           S4P43_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (362
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (50 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (362
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (50 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        512.42(4)
_cod_original_sg_symbol_Hall     -R32''-P3*2
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_original_formula_sum        'O8.00 P2 Pb3.00'
_cod_database_code               2102297
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102298
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     WC
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_chemical_formula_weight         195.86
_chemical_name_common            WC
_chemical_name_systematic        ' ?'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1
_cell_length_a                   2.8979(5)
_cell_length_b                   2.8979
_cell_length_c                   2.8289(7)
_cell_measurement_temperature    298
_cell_volume                     20.574(4)
_cod_data_source_file            ws5002.cif
_cod_database_code               2102298
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102299
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     Ni
_chemical_formula_moiety         Ni
_chemical_formula_structural     Ni
_chemical_formula_sum            Ni
_chemical_formula_weight         58.71
_chemical_name_common            Nickel
_chemical_name_systematic        ' ?'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   3.5409(5)
_cell_length_b                   3.5409
_cell_length_c                   3.5409
_cell_measurement_temperature    298
_cell_volume                     44.397(3)
_cod_data_source_file            ws5002.cif
_cod_database_code               2102299
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102300
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     'Pb2.952 Ba0.048 P2 O8'
_chemical_formula_structural     '(Pb0.984 Ba0.016)3 (PO4)2'
_chemical_formula_sum            'O8 P2 Pb3'
_chemical_formula_weight         811.54
_chemical_name_common            'Ba-doped lead phosphate'
_chemical_name_systematic        ' ?'
_space_group_IT_number           166
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            3
_cell_length_a                   5.4041(3)
_cell_length_b                   5.4041
_cell_length_c                   19.9364(15)
_cell_measurement_pressure       3290000.
_cell_measurement_temperature    298
_cell_volume                     504.22(5)
_cod_data_source_file            ws5002.cif
_cod_data_source_block           S4P55TISO_phase_1
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (136
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (6 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 

The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (136
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to /home/saulius/struct/CIF-dictionaries/cif_core.dic dictionary
named 'cif_core.dic' version 2.4.1 from 2010-06-29 (6 times).

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_Hall     -R32''-P3*2
_cod_original_sg_symbol_H-M      'R -3 m'
_cod_database_code               2102300
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102301
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     WC
_chemical_formula_structural     WC
_chemical_formula_sum            'C W'
_chemical_formula_weight         195.86
_chemical_name_common            WC
_chemical_name_systematic        ' ?'
_space_group_IT_number           187
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P -6 2'
_symmetry_space_group_name_H-M   'P -6 m 2'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1
_cell_length_a                   2.8945(7)
_cell_length_b                   2.8945
_cell_length_c                   2.8293(11)
_cell_measurement_temperature    298
_cell_volume                     20.528(5)
_cod_data_source_file            ws5002.cif
_cod_database_code               2102301
Local and long-range order in ferroelastic lead phosphate at high pressure
Angel, R. J.; Bismayer, U.; Marshall, W. G.; Acta Crystallographica Section B 60 (2004) 1–9; doi:10.1107/S0108768103026582

data_2102302
_publ_section_title
;
 Local and long-range order in ferroelastic lead phosphate at high
 pressure
;
_journal_issue                   1
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              1
_journal_page_last               9
_journal_paper_doi               10.1107/S0108768103026582
_journal_volume                  60
_journal_year                    2004
_chemical_formula_analytical     Ni
_chemical_formula_moiety         Ni
_chemical_formula_structural     Ni
_chemical_formula_sum            Ni
_chemical_formula_weight         58.71
_chemical_name_common            Nickel
_chemical_name_systematic        ' ?'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            4
_cell_length_a                   3.5355(8)
_cell_length_b                   3.5355
_cell_length_c                   3.5355
_cell_measurement_temperature    298
_cell_volume                     44.19(4)
_cod_data_source_file            ws5002.cif
_cod_database_code               2102302
Space group <i>Cc</i>: an update
Marsh, Richard E.; Acta Crystallographica Section B 60 (2004) 252–253; doi:10.1107/S0108768104003878

data_2102308
_publ_section_title
;
 Space group <i>Cc</i>: an update
;
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              252
_journal_page_last               253
_journal_paper_doi               10.1107/S0108768104003878
_journal_volume                  60
_journal_year                    2004
_chemical_formula_moiety         'C19 H21 N5'
_chemical_formula_sum            'C19 H21 N5'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_audit_creation_method           CRYM
_cell_angle_alpha                90
_cell_angle_beta                 113.92
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   31.5360
_cell_length_b                   6.4960
_cell_length_c                   17.5900
_cell_volume                     3293.958
_cod_data_source_file            bk0142.cif
_cod_data_source_block           ABORUE
_cod_depositor_comments
;
 Adding the _cell_formula_units_Z data item.

 Antanas Vaitkus,
 2017-08-05

  Added moiety chemical formula from Marsh (2004) paper.
  The summary chemical formula is calculated from moiety formula using
  AdHocParser
  (svn://www.crystallography.net/cod-tools/trunk/Formulae/AdHocParser.yp,
  revision 1441.)

  Andrius Merkys
  2013-11-11
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               2102308
Space group <i>Cc</i>: an update
Marsh, Richard E.; Acta Crystallographica Section B 60 (2004) 252–253; doi:10.1107/S0108768104003878

data_2102309
_publ_section_title
;
 Space group <i>Cc</i>: an update
;
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              252
_journal_page_last               253
_journal_paper_doi               10.1107/S0108768104003878
_journal_volume                  60
_journal_year                    2004
_chemical_formula_moiety         'C34 H32 O2 Sn'
_chemical_formula_sum            'C34 H32 O2 Sn'
_space_group_crystal_system      orthorhombic
_space_group_IT_number           43
_symmetry_space_group_name_H-M   'F d d 2'
_audit_creation_method           CRYM
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   9.6920
_cell_length_b                   67.5700
_cell_length_c                   17.0280
_cell_volume                     11151.440
_cod_data_source_file            bk0142.cif
_cod_data_source_block           ACUKIS
_cod_depositor_comments
;
 Adding the _cell_formula_units_Z data item.

 Antanas Vaitkus,
 2017-08-05

  Added moiety chemical formula from Marsh (2004) paper.
  The summary chemical formula is calculated from moiety formula using
  AdHocParser
  (svn://www.crystallography.net/cod-tools/trunk/Formulae/AdHocParser.yp,
  revision 1441.)

  Andrius Merkys
  2013-11-11
;
_cod_original_sg_symbol_H-M      Fdd2
_cod_database_code               2102309
Space group <i>Cc</i>: an update
Marsh, Richard E.; Acta Crystallographica Section B 60 (2004) 252–253; doi:10.1107/S0108768104003878

data_2102310
_publ_section_title
;
 Space group <i>Cc</i>: an update
;
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              252
_journal_page_last               253
_journal_paper_doi               10.1107/S0108768104003878
_journal_volume                  60
_journal_year                    2004
_chemical_formula_moiety         'C28 H24 N4 O8 S2 Cd'
_chemical_formula_sum            'C28 H24 Cd N4 O8 S2'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_audit_creation_method           CRYM
_cell_angle_alpha                90
_cell_angle_beta                 123.78
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   22.2330
_cell_length_b                   9.5660
_cell_length_c                   16.0170
_cell_volume                     2831.418
_cod_data_source_file            bk0142.cif
_cod_data_source_block           AFAQAZ
_cod_depositor_comments
;
 Updating space group information and adding the symmetry operation list.

 Antanas Vaitkus,
 2018-06-14

 Adding the _cell_formula_units_Z data item.

 Antanas Vaitkus,
 2017-08-05

  Added moiety chemical formula from Marsh (2004) paper.
  The summary chemical formula is calculated from moiety formula using
  AdHocParser
  (svn://www.crystallography.net/cod-tools/trunk/Formulae/AdHocParser.yp,
  revision 1441.)

  Andrius Merkys
  2013-11-11
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               2102310
Space group <i>Cc</i>: an update
Marsh, Richard E.; Acta Crystallographica Section B 60 (2004) 252–253; doi:10.1107/S0108768104003878

data_2102311
_publ_section_title
;
 Space group <i>Cc</i>: an update
;
_journal_issue                   2
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              252
_journal_page_last               253
_journal_paper_doi               10.1107/S0108768104003878
_journal_volume                  60
_journal_year                    2004
_chemical_formula_moiety         'C30 H26 N4 O4 Ni, C7 H8'
_chemical_formula_sum            'C37 H34 N4 Ni O4'
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_audit_creation_method           CRYM
_cell_angle_alpha                90
_cell_angle_beta                 120.21
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   25.2520
_cell_length_b                   9.3940
_cell_length_c                   15.3560
_cell_volume                     3147.981
_cod_data_source_file            bk0142.cif
_cod_data_source_block           BACZAH
_cod_depositor_comments
;
 Adding the _cell_formula_units_Z data item.

 Antanas Vaitkus,
 2017-08-05

  Added moiety chemical formula from Marsh (2004) paper.
  The summary chemical formula is calculated from moiety formula using
  AdHocParser
  (svn://www.crystallography.net/cod-tools/trunk/Formulae/AdHocParser.yp,
  revision 1441.)

  Andrius Merkys
  2013-11-11
;
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               2102311